Structural and electrical phase transitions in the [(C2H5)4N]2ZnI3.86Cl0.14 system
Najla Mahbouli Rhouma; Ali Rayes; Francesco Mezzadri; Davide Delmonte; Riccardi Cabassi; Gianluca Calestani; Mohamed Loukil; Journal of Solid State Chemistry 256 (2017) 60–66; doi:10.1016/j.jssc.2017.08.029

data_1560258
_publ_section_title
;
 Structural and electrical phase transitions in the
 [(C2H5)4N]2ZnI3.86Cl0.14 system
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              60
_journal_page_last               66
_journal_paper_doi               10.1016/j.jssc.2017.08.029
_journal_volume                  256
_journal_year                    2017
_chemical_formula_moiety         '2(C8 H20 N), Cl0.12 I3.88 Zn'
_chemical_formula_sum            'C16 H40 Cl0.12 I3.88 N2 Zn'
_chemical_formula_weight         822.15
_chemical_name_common
;
2(C8 H20 N), Cl0.12 I3.88 Zn
;
_space_group_crystal_system      tetragonal
_space_group_IT_number           113
_space_group_name_Hall           'P -4 2ab'
_space_group_name_H-M_alt        'P -4 21 m'
_atom_sites_solution_hydrogens   geom
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.7327(8)
_cell_length_b                   13.7327(8)
_cell_length_c                   14.7484(8)
_cell_measurement_reflns_used    213
_cell_measurement_temperature    233(2)
_cell_measurement_theta_max      18.02
_cell_measurement_theta_min      8.60
_cell_volume                     2781.4(3)
_computing_cell_refinement       'SAINT (Bruker, 2008)'
_computing_data_collection       'APEX2 (Bruker, 2008)'
_computing_data_reduction        'SAINT (Bruker, 2008)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2015b)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2015b)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015a)'
_diffrn_ambient_temperature      233(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX2 CCD'
_diffrn_measurement_method       '\w scan'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0454
_diffrn_reflns_av_unetI/netI     0.0189
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            31860
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.489
_diffrn_reflns_theta_min         1.381
_exptl_absorpt_coefficient_mu    5.158
_exptl_absorpt_correction_T_max  0.233
_exptl_absorpt_correction_T_min  0.156
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2008)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.954
_exptl_crystal_description       block
_exptl_crystal_F_000             1544
_exptl_crystal_size_max          0.380
_exptl_crystal_size_mid          0.380
_exptl_crystal_size_min          0.280
_refine_diff_density_max         0.714
_refine_diff_density_min         -0.677
_refine_diff_density_rms         0.078
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.48(7)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.094
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     144
_refine_ls_number_reflns         2772
_refine_ls_number_restraints     54
_refine_ls_restrained_S_all      1.101
_refine_ls_R_factor_all          0.0321
_refine_ls_R_factor_gt           0.0304
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0312P)^2^+3.4713P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0698
_refine_ls_wR_factor_ref         0.0708
_reflns_Friedel_coverage         0.777
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                2668
_reflns_number_total             2772
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            JSSC-2017-256-60-2.cif
_cod_data_source_block           O_233
_cod_original_cell_volume        2781.4(4)
_cod_database_code               1560258
_shelx_estimated_absorpt_t_min   0.245
_shelx_estimated_absorpt_t_max   0.326
_shelx_res_checksum              4989
_shelx_hkl_checksum              92172